At the conclusion of this block the student will understand: * How to use asphalt binder specifications * The limitations of these specifications which led to the development of new asphalt binder specifications This material is covered in detail in Chapter 2 “Asphalt Binder Refining, Uses, and Properties” in the recommended text book.
The first paved roadway in the United States was Pennsylvania Avenue in front of the White House. This pavement was constructed with an asphalt binder product quarried from a naturally occurring “lake” of asphalt on the island of Trinidad off the coast of Venezuela. A second source of this type of asphalt binder product can be found in Bermudez, Venezuela. These products are still used today. In fact, a Trinidad lake asphalt was placed near Mobile, Alabama in July, 1998. Each lake asphalt has consistent but different amounts of bitumen, inorganic material. Because of these consistent differences, the amount of solvent-insoluble inorganic material is one common method used to identify and specify the lake asphalt source. This solubility test was used in all subsequent asphalt binder specifications throughout the 20 th century.
During the late 1800's and early 1900's the demand for paved roads increased so fast that the time-intensive processing and shipping of lake asphalt was limiting the miles of paved roads constructed each year. This led to the increasing use of petroleum refinery-based asphalt binders. It is interesting to note that these asphalt binders were originally considered inferior to lake asphalt because of their crude source-dependent material properties.
Replica of the engine house and derrick at Oil Creek PA. On August 28, 1859, George Bissell and Edwin L. Drake made the first successful use of a drilling rig on a well drilled especially to produce oil, at a site on Oil Creek near Titusville, Pennsylvania. The Drake well is often referred to as the "first" commercial oil well. However, before the Drake well, oil-producing wells in the United States were wells that were drilled for salt brine, and produced oil and gas only as accidental byproducts. Historians have noted that the importance of the Drake well was not in being the first well to produce oil, but in attracting the first great wave of investment in oil drilling, refining, and marketing: "The importance of the Drake well was in the fact that it caused prompt additional drilling, thus establishing a supply of petroleum in sufficient quantity to support business enterprises of magnitude.
A number of products are obtained from one barrel of crude. Asphalt binder is what is left after the more volatile products are removed and it is commonly referred to as the “bottom of the barrel”.
In order to purchase a product, the desirable characteristics and important material properties must be known. When these parameters are presented in written form, they are called specifications.
The first approach to characterizing the stiffness of an asphalt binder was to chew on it. An engineer would take a small sample of material, roll it into a ball, and place it between their teeth. The pressure required to deform the ball was considered an indication of the stiffness of the asphalt binder. However, this method was very subjective and could not be used to routinely specify the particular requirements of an asphalt binder for a given construction project. These drawbacks eventually led to the development of the penetration test.
The penetration test started out using a No. 2 sewing machine needle mounted on a shaft for a total mass of 100 g. This needle was allowed to sink into (penetrate) a container of asphalt binder at room temperature (25 o C) for 5 seconds. The consistency (stiffness) of a given asphalt binder was reported as the depth in tenths of a millimeter (dmm) that the needle penetrated the asphalt binder.
This test was used to standardize the penetration grading system approach for specifying asphalt binders. This specification uses the penetration of the original asphalt binder in the grade names. That is, a 120-150 penetration grade asphalt binder will have a penetration value for the original asphalt binder of between 120 and 150 tenths of a millimeter.
Other tests have been added to address safety issues (the flash point test), the ability of the asphalt binder to deform without breaking (ductility test), and the influence of heat hardening on asphalt binder properties (thin film oven test).
If an asphalt binder is heated to a high enough temperature, it gives off sufficient vapors to flash (ignite) in the presence of a spark or open flame. The Cleveland Open Cup test determines the temperature at which this flash occurs. In this test, a small sample of asphalt binder is poured into the brass cup which is placed over an electric heater. A thermometer is submerged to a prescribed depth into the asphalt and used to monitor the temperature rise. When the temperature gets close to the suspected flash point, the gas line is turned on and a small flame lit at the end of the wand. The flash point is the temperature at which a small blue flicker around the inside of the cup is seen as the wand is passed horizontally over the surface of the cup.
This test evaluates the ability of an asphalt binder sample to stretch at a rate of 5 cm/min at 25 o C. The distance the samples can be pulled is measured directly from the centimeter scale mounted to the top of the tank. The significance of the ductility test to indicate performance-related properties has been debated for a number of years due to its empirical nature and poor reproducibility of test results. In general, asphalts binder with lower ductility have a greater tendency to produce pavements which have excessive cracking
A sample of asphalt binder is dissolved in a solvent then filtered through a Gooch crucible mounted in the top of a vacuum flask. The amount of insoluble material retained on the filter represents the impurities in the asphalt binder.
Thin film oven aging is a laboratory procedure for simulating the change in asphalt binder properties which occur during tank storage, mixing and construction processes. This test can also be used to measure the loss of volatiles in the asphalt binder by determining the percent difference in the mass before and after aging. A 50 g sample of asphalt binder is poured into each of three flat-bottomed pans. This results in a layer of asphalt binder of about 3.2 mm deep. Three pans are placed on a rotating shelf in a 163 o C oven for 5 hours. The aged samples are then combined into one container, mixed, and used to determine the aged asphalt binder properties.
There are five penetration grades of asphalt binder with discrete ranges. That is, there is no overlap in penetration values between grades. It is possible to have an asphalt binder which will not meet any penetration grading requirement. This table presents two of these grades. Note the flash point decreases with increasing penetration. This is because softer asphalt binders usually have a higher percentage of lighter ends which will “flash” at lower temperatures. The specification allows for this difference. Since these fractions of the asphalt binder are also easily removed by heating, this means that there will be a higher percentage mass loss on aging. This greater loss of the softer asphalt components is reflected in the differences in requirements on the percent of the original penetration retained after aging. That is, the more light ends lost during aging, the greater the stiffening affect due to aging. This loss of the softer asphalt binder components is also reflected the ductility requirements.
Temperature susceptibility (i.e., the rate of change in material properties with a change in temperature) can be estimated by determining the penetration at two (or more) temperatures. The most commonly used temperatures are 4 and 25 o C with a 100 g load for 5 seconds. This figure highlights one of the major problems with the penetration grading system. For example, three sources of asphalt binder can have the same penetration at 25 o C but decidedly different properties above and below this temperature. This helps explain the differences in observed pavement performances even though the same penetration grade of asphalt binder is specified.
Several advantages are responsible for the penetration specifications being widely used throughout the 20 th century. For instance, as late as 1995 the Minnesota Department of Transportation was still using this specification to purchase asphalt binder. These advantages include an estimate of material properties at the average in-service temperature (i.e, the average between summer highs and winter lows), low cost of the equipment, simplicity, and short testing times needed to obtain results.
However, there are several disadvantages associated with penetration specifications. These include allowing a wide range of material properties at high and low temperatures for a given penetration grade, variable shear rates (i.e., the needle will penetrate the asphalt faster for softer as compared to harder asphalts), lack of fundamental measurements needed for mechanistic pavement performance prediction models (i.e., no stress or strain measurements), their inability to evaluate shear rate dependent materials (e.g., polymer modified asphalt binders), and lack of information for selecting appropriate mixing and compaction temperatures (necessary information for preparing mixtures in the laboratory and plant).
These disadvantages led to the development of the viscosity grading system in the 1970's which is detailed in ASTM D3381. This one ASTM standard actually contains three separate specifications designated as: Table 1, Table 2, and Table 3. The first two specifications are based on the original properties of the asphalt while the last table is based on the properties of the asphalt binder after rolling thin film oven aging. Each of these tables and differences between them will be discussed in the following slides. In the early 1960s an improved asphalt grading system was developed that incorporated a rational scientific viscosity test. This scientific test replaced the empirical penetration test as the key asphalt binder characterization. Viscosity grading quantifies the following asphalt binder characteristics: Viscosity grading can be done on original (as-supplied) asphalt binder samples (called AC grading) or aged residue samples (called AR grading). The AR viscosity test is based on the viscosity of aged residue from the rolling thin film oven test. With AC grading, the asphalt binder is characterized by the properties it possesses before it undergoes the HMA manufacturing process. The AR grading system is an attempt to simulate asphalt binder properties after it undergoes a typical HMA manufacturing process and thus, it should be more representative of how asphalt binder behaves in HMA pavements. Table 1 lists key advantages and disadvantages of the viscosity grading system. Advantages Unlike penetration depth, viscosity is a fundamental engineering parameter. Test temperatures correlate well with: • 25° C (77° F) – average pavement temp. • 60° C (140° F) – high pavement temp. • 135° C (275° F) – HMA mixing temp. Temperature susceptibility (the change in asphalt binder rheology with temperature) can be somewhat determined because viscosity is measured at three different temperatures (penetration only is measured at 25° C (77° F)). Testing equipment and standards are widely available Disadvantages The principal grading (done at 25° C (77° F)) may not accurately reflect low-temperature asphalt binder rheology. When using the AC grading system, thin film oven test residue viscosities can vary greatly with the same AC grade. Therefore, although asphalt binders are of the same AC grade they may behave differently after construction. The testing is more expensive and takes longer than the penetration test. .
Viscosity is shear stress divided by the shear strain rate. These units of measurement provide at least a limited estimate of fundamental material properties. The easiest way to picture shear is to visualize a deck of cards which have a vertical line marked on the side. As pressure is applied to the top of the deck, the cards slide over one another and the marked dots on the individual cards start to separate. The shear rate is the rate at which these dots separate.
Two viscosity measurements are used in this specification: Absolute viscosity (60 o C) and kinematic viscosity (135 o C). Both use the principle of the rate of flow through a known area to measure viscosity. Because asphalt binder is still very thick (stiff) at 60 o C, a vacuum is needed to move the asphalt through the tube in a reasonable time. At 135 o C, gravity and a falling head pressure is sufficient to get the asphalt binder to flow.
At the 60 o C test temperature, the tube is charged at 135 o C and then placed in the test temperature bath. The tube temperature is allowed to equalize with the bath temperature, a vacuum line is attached to the top of the small diameter tube, and the flow is started. The time it takes the asphalt to flow past the timing marks times the tube calibration constant gives the viscosity of the asphalt binder in Poise.
The tube is charged in the 135 o C bath and left for about 20 minutes. A vacuum line is touched briefly to the top of the small diameter tube until the asphalt binder moves over the upper hump in the tube. The time it takes the asphalt binder to flow past the timing marks times the tube calibration constant gives the viscosity of the asphalt in centistoke. Centistokes are converted to centipoise by mulitplying centistokes by the specific gravity of the asphalt binder.
All three of the viscosity graded asphalt binder specifications are listed in ASTM D3381. The first two specifications are based on the viscosity of the original asphalt binder at 60 o C. The third specification is based on the viscosity of the rolling thin film oven aged residue at 60 o C.
Requirements on both the absolute and kinematic viscosities are set in these specifications. The grading system is based on the absolute viscosity (60 o C). A minimum viscosity at 135 o C is included to help define the maximum rate of change of material properties with temperature. A minimum penetration value is also included in these specifications as a means limiting temperature susceptibility. The penetration values decreases with increasing viscosity. In other words, the stiffer the asphalt binder, the less distance the needle will penetrate into the asphalt binder. As with the penetration specifications, requirements for safety and limits on aging of the asphalt binder during construction are included. The flash point temperature requirements increase with increasing viscosity (less volatiles with increasing viscosity). Maximum limits on viscosity after thin film oven aging limit the amount of acceptable aging during mixing and construction.
Table 2 viscosity specifications are very similar to Table 1 specifications with two exceptions: Table 2 specifications allow for an AC 30 grade, and Table 2 asphalt binders are required to be less temperature susceptible.
This table compares two of the viscosity graded Table 1 specifications. The viscosity grading system provides immediate information as to the mean anticipated viscosity at 60 o C. For example, an AC 25 will have a mean viscosity of 250 Poise (2.5 times 100). Because of the limited allowable range (coefficient of variance of 20 percent), there is no overlap between the AC grades.
All of the same tests are used to specific Table 1 and Table 2 specifications. The differences between the two specifications are highlighted in this example. While the original and maximum aged viscosities at 60 o C remain the same for both tables, the minimum requirements for the 135 o C viscosity and penetrations are increased. There is also an increase in the required ductility after aging for the harder (higher viscosity) asphalt binders.
This figure demonstrates the differences between a Table 1 and a Table 2 AC 20. Both asphalt binders can have similar viscosities at 60 o C. The minimum 135 o C for the Table 1 AC 20 is 210 centistokes. This minimum limits the steepness of the viscosity temperature line (i.e., puts a maximum on the temperature susceptibility. The higher minimum requirement (300 centistokes) for the Table 2 AC 20 further limits this slope. The minimum penetration value places a limit on maximum stiffness of the asphalt binder at 25 o C. Remember that higher penetration numbers represent lower asphalt binder stiffness. The higher minimum requirement for the Table 2 AC 20 also results in a shallower maximum slope. Neither Table 1 or Table 2 specifications place any lower limit on the rate of change in properties with temperature. This means that the pavement performance of a given AC 20 can still vary widely.
Information from this testing can be used to estimate appropriate mixing and compaction temperatures. This is accomplished by graphing viscosity in Poise (on a log scale of the y-axis) versus temperature (arithmetic scale on the x-axis). The mixing temperature is selected so that an equal viscosity is achieved. Based on historical experience, a viscosity of 1.7 + 0.2 Poise is used. The temperature at which the viscosity is 2.8 + 0.3 is used to select the compaction temperature.
Advantages to using viscosity specifications include measurements with engineering units, limits on maximum temperature susceptibility and changes in properties due to aging, and information can be obtained on appropriate mixing and compaction temperatures.
Disadvantages include the higher cost of the more sophisticated equipment and glassware required for viscosity tests, longer testing times, increased training needed for technicians, the lack of lower limits for temperature susceptibility, and the inability of these viscosity measurements for assessing non-Newtonian (shear rate dependent) properties.
The rolling thin film oven places 35 g of asphalt binder in glass jars which are then anchored in a rotating carriage. As the carriage rotates, the asphalt binder rolls around the inside of jar and air is blown over the surface each time the jar passes the air nozzle at the bottom of the oven. This continually exposes a new surface of asphalt binder to the effects of air and heat. This test is run at 163 o C for 80 minutes. At the end of this time, the asphalt binder is scraped out of the jars and combined into one container, stirred, and used to determine the effects of oxidation and heat aging on viscosity, penetration, and ductility.
The allowable range of RTFO aged viscosities is greater than those for the AC viscosity designations. The coefficient of variation is 25 percent. The only tests which are conducted on the original asphalt binder are flash point and penetration (so that the percent of original penetration can be calculated).
The main advantage to this specification is that it is based on the properties of the asphalt binder behind the paver. That is, it is based on the in-place asphalt binder properties at the time the roadway is opened to traffic. Other advantages to using the AR specification are similar to those for the first two viscosity specifications.
Disadvantages include a problem with a lack of wide-spread experience in determining desirable properties, longer times before results can be reported because the material has to be aged prior to testing, and other disadvantages as seen in the previous viscosity grading specifications.
This figure provides a general comparison of the various traditional specifications. While there is no direct relationship between the specifications, there is a general relationship between stiffness and viscosity. Higher penetration numbers correspond with lower viscosities.
Block 2 history and background 13
Senior/Graduate HMA Course Asphalt Binders Background History of SpecificationsAsphalt Binders History and Background 1
Background First US Hot Mix Asphalt (HMA) constructed in 1870’s – Pennsylvania Ave. – Used naturally occurring asphalt binders from surface of lake on Island of Trinidad Two sources – Island of Trinadad – Bermudez, Venezuela
BackgroundEach lake asphalt source very consistent – Used solubility test to determine source » Insolubles differed substantially between sourcesDemand for paved roads exceeded the supply oflake asphalts in late 1800’s – Led to use of petroleum asphalts bindersAsphalt Binder History and Background 5
Petroleum-Based Asphalt BindersAsphalt binder is waste product from refineryprocessing of crude oil – Sometimes called the “bottom of the barrel”Properties depend on: – Refinery operations – Composition crude source-dependent Gasoline Kerosene Lt. Gas Oil Barrel of Crude Oil Diesel Motor Oils Asphalt Asphalt Binder History and Background 7
Purchasing of Asphalt Binders Need to be able to specify desirable characteristics “Desirable characteristics” have evolved over time and with increasing technological advances Purchasing requires specificationsAsphalt Binder History and Background 8
Early SpecificationsLake Asphalts – Appearance – Solubility in carbon disulfidePetroleum asphalt binders (early 1900’s) – Consistency » Chewing » Penetration machine Measure consistencyAsphalt Binder History and Background 9
Penetration TestingSewing machine needleSpecified load, time, temperature100 g Penetration in 0.1 mm Initial After 5 seconds
Penetration Specification Five Grades • 40 - 50 • 60 - 70 • 85 - 100 • 120 - 150 • 200 - 300Asphalt Binder History and Background 11
Penetration Gradation Specification Uses penetration results to specify Adds – Flash point test – Ductility – Solubility – Thin film oven aging » Penetration » Ductility Asphalt Binder History and Background 12
Flash Point (Safety) Thermometer Cup filled with asphalt binder Wand attached to gas lineAsphalt Binder History and Background 13
DuctilityAsphalt Binder History and Background 14
Solubility (Purity)Asphalt Binder History and Background 15
Thin Film Oven Pan ThermometerOutside of Oven Rotating Shelf Asphalt Binder History and Background 16
Typical Penetration SpecificationsPenetration 40 - 50 200 - 300Flash Point, F 450+ 350+Ductility, cm 100+ 100+Solubility, % 99.0+ 99.0+Retained Pen., % 55+ 37+Ductility, cm NA 100+ Asphalt Binder History and Background 17
MediumPenetration, 0.1 mm Low High 25C (77F) Temperature Asphalt Binder History and Background 18
AdvantagesGrades asphalt binders near average in-service temp.FastCan be used in field labsLow capital costsPrecision well establishedTemp. susceptibility can be determined Asphalt Binder History and Background 19
DisadvantagesEmpirical testShear rate – High – VariableMixing and compaction temp. information notavailableSimilar penetrations at 25C (77F) do notreflect wide differences in asphaltsAsphalt Binder History and Background 20
Viscosity Graded SpecificationsAsphalt Binder History and Background 21
DefinitionViscosity: the ratio between the applied shearstress and the rate of shear. η=τ/γ Asphalt Binder History and Background 22
Types of Viscosity Tubes Zietfuchs Cross-Arm Asphalt Institute Tube TubeAsphalt Binder History and Background 23
TestingAbsolute viscosity – U-shaped tube with timing marks & filled with asphalt binder – Placed in 60C bath – Vacuum used to pull asphalt through tube – Time to pass marks – Visc. in Pa s (Poise) Asphalt Binder History and Background 24
Testing Kinematic viscosity – Cross arm tube with timing marks & filled with asphalt – Placed in 135C bath – Once started gravity moves asphalt through tube – Time to pass marks – Visc. in mm2 / s (centistoke)Asphalt Binder History and Background 25
Viscosity Grade Specifications ASTM D3381 Three specifications – Table 1 » Original properties – Table 2 » Original properties – Table 3 » Rolling thin film oven agingAsphalt Binder History and Background 26
Table 1 & 2 Tests Viscosities at 60 and 135oC Penetrations at 25oC Flash point Solubility TFO aged residue – Viscosity at 60oC – Ductility at 25oCAsphalt Binder History and Background 27
Table 1 & 2 GradesTable 1 – AC 2.5, AC 5, AC 10, AC 20, AC 40Table 2 – AC 2.5, AC 5, AC 10, AC 20, AC 30, AC 40Asphalt Binder History and Background 28
Table 1 Example AC 2.5 AC 40Visc, 60C 250 + 50 4,000 + 800Visc, 135C 80+ 300+Penetration 200+ 20+Visc, 60C <1,250 <20,000Ductility 100+ 10+ Asphalt Binder History and Background 29
Table 2 Example AC 2.5 AC 40Visc, 60C 250 + 50 4,000 + 800Visc, 135C 125+ 400+Penetration 220+ 40+Visc, 60C <1,250 <20,000Ductility 100+ 25+ Asphalt Binder History and Background 30
Ave. Mixing Hot Service & Summer Temp. CompactionViscosity (Stiffness) 40 Pen 60 Pen 2400 Low 1600 Table 2 300 210 Table 1 25C (77F) 60C (140F) 135C (275F) Temperature Asphalt Binder History and Background 31
Mixing/Compaction TempsViscosity, Pa s 10 5 1 .5 .3 Compaction Range .2 Mixing Range .1 100 110 120 130 140 150 160 170 180 190 200 Temperature, C Asphalt Binder History and Background 32
Advantages (Original AC Visc. Grade) Fundamental property Wide range of temperatures Based on max. pavement surface temp. Wide range of instruments Test method precision established Temperature susceptibility is controlled Limits aging Information on mixing & compaction temps.Asphalt Binder History and Background 33
Disadvantages (Original AC Visc. Grade)More expensiveLonger testing timeMore technician skill neededNot applicable for Non-Newtonian materialsWide range of properties for same gradeAsphalt Binder History and Background 34
Table 3 AR Grades – AR 1000, AR 2000, AR 4000, AR 8000, AR 16000 Tests on RTFO aged residue – Viscosities at 60 and 135oC – Penetrations at 25oC – % of Original Penetration – Ductility – Properties of unaged asphalt binders » Flash point and solubilityAsphalt Binder History and Background 35
Rolling Thin Film OvenAsphalt Binder History and Background 36
Table 3 Specification AR 1000 AR 16,000Visc, 60C 1,000 + 250 16,000 + 4,000Visc, 135C 140+ 550+Pen. 65+ 20+% Orig. Pen NS 52+ Asphalt Binder History and Background 37
Advantages (AR Visc. Grade) Represents asphalt binder properties after mixing Fundamental properties Covers wide range of temperatures Limits agingAsphalt Binder History and Background 38
Disadvantages (AR Visc. Grade)Highly regionalRequires different testing equipmentLonger testing timeNo consistency test on original Asphalt BinderNot applicable for Non-Newtonian materialsWide range of properties for same gradeAsphalt Binder History and Background 39
Penetration Grades AC 40 AR 16000 40Viscosity, 60C (140F) 100 50 AC 20 AR 8000 60 50 AC 10 70 AR 4000 85 100 AC 5 AR 2000 120 150 AC 2.5 10 200 AR 1000 300 5 Asphalt Binder History and Background 40
QUESTIONS?Asphalt Binder History and Background 41